اکسید آهن(II,III) (به انگلیسی: Iron(II,III) oxide) یک ترکیب شیمیایی با شناسه پابکم ۱۶۲۱۱۹۷۸ و جرم مولی 231.533 g/mol بوده و شکل ظاهری این ترکیب، پودری سیاه رنگ است. فرمول کلی این ترکیب Fe3O4 است. دو ترکیب دیگر، یکی اکسید آهن دو ظرفیتی(FeO)، ترکیبی کمیاب بوده و دیگری اکسید آهن سه ظرفیتی با فرمول (Fe2O3) در شیمی به نام هماتیت معروف است و در متنهای کهن فارسی به نام شادنه آمده است.
Iron(II,III) oxide is the chemical compound with formula Fe3O4. It occurs in nature as the mineral magnetite. It is one of a number of iron oxides, the others being iron(II) oxide (FeO), which is rare, and iron(III) oxide (Fe2O3) also known as hematite. It contains both Fe2+ and Fe3+ ions and is sometimes formulated as FeO ∙ Fe2O3. This iron oxide is encountered in the laboratory as a black powder. It exhibits permanent magnetism and is ferrimagnetic, but is sometimes incorrectly described as ferromagnetic. Its most extensive use is as a black pigment. For this purpose, it is synthesised rather than being extracted from the naturally occurring mineral as the particle size and shape can be varied by the method of production.
The well-crystallized magnetite (Fe3O4) is thermodynamically more stable than the ferrous hydroxide (Fe(OH)2 ).
Magnetite can be prepared in the laboratory as a ferrofluid in the Massart method by mixing iron(II) chloride and iron(III) chloride in the presence of sodium hydroxide. Magnetite can also be prepared by the chemical co-precipitation in presence of ammonia, which consist in a mixture of a solution 0.1 M of FeCl3·6H2O and FeCl2·4H2O with mechanic agitation of about 2000 rpm. The molar ratio of FeCl3:FeCl2 can be 2:1; heating this solution at 70 °C, and immediately the speed is elevated to 7500 rpm and adding quickly a solution of NH4OH (10 volume %), immediately a dark precipitate will be formed, which consists of nanoparticles of magnetite. In both cases, the precipitation reaction rely on a quick transformation of acidic hydrolyzed iron ions into the spinel iron oxide structure, by hydrolysis at elevated pH values (above ca. 10).
Considerable efforts has been devoted towards controlling the particle formation process of magnetite nanoparticles due to the challenging and complex chemistry reactions involved in the phase transformations prior to the formation of the magnetite spinel structure. Magnetite particles are of interests in bioscience applications such as in magnetic resonance imaging (MRI) since iron oxide magnetite nanoparticles represent a non-toxic alternative to currently employed gadolinium-based contrast agents. However, due to lack of control over the specific transformations involved in the formation of the particles, truly superparamagnetic particles have not yet been prepared from magnetite, i.e. magnetite nanoparticles that completely lose their permanent magnetic characteristic in the absence of an external magnetic field (which by definition show a coercivity of 0 A/m). The smallest values currently reported for nanosized magnetite particles is Hc = 8.5 A m−1, whereas the largest reported magnetization value is 87 Am2 kg−1 for synthetic magnetite.
Pigment quality Fe3O4, so called synthetic magnetite, can be prepared using processes that use industrial wastes, scrap iron or solutions containing iron salts (e.g. those produced as by-products in industrial processes such as the acid vat treatment (pickling) of steel):
Oxidation of Fe metal in the Laux process where nitrobenzene is treated with iron metal using FeCl2 as a catalyst to produce aniline:
C6H5NO2 + 3 Fe + 2 H2O → C6H5NH2 + Fe3O4
Oxidation of FeII compounds, e.g. the precipitation of iron(II) salts as hydroxides followed by oxidation by aeration where careful control of the pH determines the oxide produced.
Production of nano-particles can be performed chemically by taking for example mixtures of FeII and FeIII salts and mixing them with alkali to precipitate colloidal Fe3O4. The reaction conditions are critical to the process and determine the particle size.
Reduction of magnetite ore by CO in a blast furnace is used to produce iron as part of steel production process:
Fe3O4 has a cubic inverse spinel group structure which consists of a cubic close packed array of oxide ions where all of the Fe2+ ions occupy half of the octahedral sites and the Fe3+ are split evenly across the remaining octahedral sites and the tetrahedral sites.
Both FeO and γ-Fe2O3 have a similar cubic close packed array of oxide ions and this accounts for the ready interchangeability between the three compounds on oxidation and reduction as these reactions entail a relatively small change to the overall structure. Fe3O4 samples can be non-stoichiometric.
The ferrimagnetism of Fe3O4 arises because the electron spins of the FeII and FeIII ions in the octahedral sites are coupled and the spins of the FeIII ions in the tetrahedral sites are coupled but anti-parallel to the former. The net effect is that the magnetic contributions of both sets are not balanced and there is a permanent magnetism.
Fe3O4 is ferrimagnetic with a Curie temperature of 858 K. There is a phase transition at 120K, called Verwey transition where there is a discontinuity in the structure, conductivity and magnetic properties. This effect has been extensively investigated and whilst various explanations have been proposed, it does not appear to be fully understood.
Fe3O4 is an electrical conductor with a conductivity significantly higher (X 106) than Fe2O3, and this is ascribed to electron exchange between the FeII and FeIII centres.
Fe3O4 is used as a black pigment and is known as C.I pigment black 11 (C.I. No.77499) or Mars Black.
^Massart, R. (1981). "Preparation of aqueous magnetic liquids in alkaline and acidic media". IEEE Transactions on Magnetics. 17 (2): 1247–1248. doi:10.1109/TMAG.1981.1061188.
^Keshavarz, Sahar; Xu, Yaolin; Hrdy, Spencer; Lemley, Clay; Mewes, Tim; Bao, Yuping (2010). "Relaxation of Polymer Coated Fe3O4 Magnetic Nanoparticles in Aqueous Solution". IEEE Transactions on Magnetics. 46 (6): 1541–1543. doi:10.1109/TMAG.2010.2040588.
^Jolivet, Jean-Pierre; Chanéac, Corinne; Tronc, Elisabeth (2004). "Iron oxide chemistry. From molecular clusters to extended solid networks". Chemical Communications (5): 477–483. doi:10.1039/B304532N.
^Ström, Valter; Olsson, Richard T.; Rao, K. V. (2010). "Real-time monitoring of the evolution of magnetism during precipitation of superparamagnetic nanoparticles for bioscience applications". Journal of Materials Chemistry. 20 (20): 4168. doi:10.1039/C0JM00043D.
^Fang, Mei; Ström, Valter; Olsson, Richard T.; Belova, Lyubov; Rao, K. V. (2011). "Rapid mixing: A route to synthesize magnetite nanoparticles with high moment". Applied Physics Letters. 99 (22): 222501. doi:10.1063/1.3662965.
^Fang, Mei; Ström, Valter; Olsson, Richard T; Belova, Lyubov; Rao, K. V. (2012). "Particle size and magnetic properties dependence on growth temperature for rapid mixed co-precipitated magnetite nanoparticles". Nanotechnology. 23 (14): 145601. doi:10.1088/0957-4484/23/14/145601.
^US patent 2596954, 1947, Process for reduction of iron ore to magnetiteHeath T.D.
^Hanzlik M.; Heunemann C.; Holtkamp-Rötzler E.; Winklhofer M.; Petersen N.; Fleissner G (2000). "Superparamagnetic Magnetite in the Upper Beak Tissue of Homing Pigeons". BioMetals. 13 (4): 325–331. doi:10.1023/A:1009214526685. PMID11247039.